#------------------------------------------------------------------------------
#$Date: 2016-02-18 17:37:37 +0200 (Thu, 18 Feb 2016) $
#$Revision: 176729 $
#$URL: svn://www.crystallography.net/cod/cif/1/50/80/1508096.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1508096
loop_
_publ_author_name
'Inokuma, Yasuhide'
'Arai, Tatsuhiko'
'Fujita, Makoto'
_publ_contact_author             'Makoto Fujita'
_publ_section_title
;
 Networked molecular cages as crystalline sponges for fullerenes and other
 guests.
;
_journal_issue                   9
_journal_name_full               'Nature chemistry'
_journal_page_first              780
_journal_page_last               783
_journal_paper_doi               10.1038/nchem.742
_journal_volume                  2
_journal_year                    2010
_chemical_formula_moiety         'C26 H16 Co N10 S2'
_chemical_formula_sum            'C26 H16 Co N10 S2'
_chemical_formula_weight         591.56
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           225
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            24
_cell_length_a                   37.461(5)
_cell_length_b                   37.461(5)
_cell_length_c                   37.461(5)
_cell_measurement_reflns_used    8849
_cell_measurement_temperature    90(2)
_cell_measurement_theta_max      23.19
_cell_measurement_theta_min      2.37
_cell_volume                     52570(12)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      90(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0752
_diffrn_reflns_av_sigmaI/netI    0.0175
_diffrn_reflns_limit_h_max       41
_diffrn_reflns_limit_h_min       -41
_diffrn_reflns_limit_k_max       41
_diffrn_reflns_limit_k_min       -41
_diffrn_reflns_limit_l_max       41
_diffrn_reflns_limit_l_min       -40
_diffrn_reflns_number            97091
_diffrn_reflns_theta_full        23.45
_diffrn_reflns_theta_max         23.45
_diffrn_reflns_theta_min         1.54
_exptl_absorpt_coefficient_mu    0.255
_exptl_absorpt_correction_T_max  0.9367
_exptl_absorpt_correction_T_min  0.9161
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    0.448
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       cubic
_exptl_crystal_F_000             7224
_exptl_crystal_size_max          0.35
_exptl_crystal_size_mid          0.31
_exptl_crystal_size_min          0.26
_platon_squeeze_details
;
;
_refine_diff_density_max         0.389
_refine_diff_density_min         -0.417
_refine_diff_density_rms         0.048
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   2.013
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     58
_refine_ls_number_reflns         1954
_refine_ls_number_restraints     12
_refine_ls_restrained_S_all      2.138
_refine_ls_R_factor_all          0.1286
_refine_ls_R_factor_gt           0.0998
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2830
_refine_ls_wR_factor_ref         0.2978
_reflns_number_gt                1443
_reflns_number_total             1954
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            nchem.742-s2.cif
_cod_data_source_block           fm3m
_cod_original_cell_volume        52571(12)
_cod_database_code               1508096
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'x, z, y'
'y, -z, x'
'y, x, -z'
'x, -z, y'
'-z, y, x'
'z, x, -y'
'y, z, -x'
'z, y, -x'
'-z, x, -y'
'x, z, -y'
'y, -z, -x'
'x, -z, -y'
'-z, y, -x'
'x, -y, z'
'y, -x, z'
'x, -y, -z'
'y, -x, -z'
'-y, -z, -x'
'-x, -y, z'
'-y, -x, -z'
'-z, -x, -y'
'-z, -y, -x'
'z, -x, -y'
'x, y+1/2, z+1/2'
'x, z+1/2, y+1/2'
'y, -z+1/2, x+1/2'
'y, x+1/2, -z+1/2'
'x, -z+1/2, y+1/2'
'-z, y+1/2, x+1/2'
'z, x+1/2, -y+1/2'
'y, z+1/2, -x+1/2'
'z, y+1/2, -x+1/2'
'-z, x+1/2, -y+1/2'
'x, z+1/2, -y+1/2'
'y, -z+1/2, -x+1/2'
'x, -z+1/2, -y+1/2'
'-z, y+1/2, -x+1/2'
'x, -y+1/2, z+1/2'
'y, -x+1/2, z+1/2'
'x, -y+1/2, -z+1/2'
'y, -x+1/2, -z+1/2'
'-y, -z+1/2, -x+1/2'
'-x, -y+1/2, z+1/2'
'-y, -x+1/2, -z+1/2'
'-z, -x+1/2, -y+1/2'
'-z, -y+1/2, -x+1/2'
'z, -x+1/2, -y+1/2'
'x+1/2, y, z+1/2'
'x+1/2, z, y+1/2'
'y+1/2, -z, x+1/2'
'y+1/2, x, -z+1/2'
'x+1/2, -z, y+1/2'
'-z+1/2, y, x+1/2'
'z+1/2, x, -y+1/2'
'y+1/2, z, -x+1/2'
'z+1/2, y, -x+1/2'
'-z+1/2, x, -y+1/2'
'x+1/2, z, -y+1/2'
'y+1/2, -z, -x+1/2'
'x+1/2, -z, -y+1/2'
'-z+1/2, y, -x+1/2'
'x+1/2, -y, z+1/2'
'y+1/2, -x, z+1/2'
'x+1/2, -y, -z+1/2'
'y+1/2, -x, -z+1/2'
'-y+1/2, -z, -x+1/2'
'-x+1/2, -y, z+1/2'
'-y+1/2, -x, -z+1/2'
'-z+1/2, -x, -y+1/2'
'-z+1/2, -y, -x+1/2'
'z+1/2, -x, -y+1/2'
'x+1/2, y+1/2, z'
'x+1/2, z+1/2, y'
'y+1/2, -z+1/2, x'
'y+1/2, x+1/2, -z'
'x+1/2, -z+1/2, y'
'-z+1/2, y+1/2, x'
'z+1/2, x+1/2, -y'
'y+1/2, z+1/2, -x'
'z+1/2, y+1/2, -x'
'-z+1/2, x+1/2, -y'
'x+1/2, z+1/2, -y'
'y+1/2, -z+1/2, -x'
'x+1/2, -z+1/2, -y'
'-z+1/2, y+1/2, -x'
'x+1/2, -y+1/2, z'
'y+1/2, -x+1/2, z'
'x+1/2, -y+1/2, -z'
'y+1/2, -x+1/2, -z'
'-y+1/2, -z+1/2, -x'
'-x+1/2, -y+1/2, z'
'-y+1/2, -x+1/2, -z'
'-z+1/2, -x+1/2, -y'
'-z+1/2, -y+1/2, -x'
'z+1/2, -x+1/2, -y'
'-x, -y, -z'
'-x, -z, -y'
'-y, z, -x'
'-y, -x, z'
'-x, z, -y'
'z, -y, -x'
'-z, -x, y'
'-y, -z, x'
'-z, -y, x'
'z, -x, y'
'-x, -z, y'
'-y, z, x'
'-x, z, y'
'z, -y, x'
'-x, y, -z'
'-y, x, -z'
'-x, y, z'
'-y, x, z'
'y, z, x'
'x, y, -z'
'y, x, z'
'z, x, y'
'z, y, x'
'-z, x, y'
'-x, -y+1/2, -z+1/2'
'-x, -z+1/2, -y+1/2'
'-y, z+1/2, -x+1/2'
'-y, -x+1/2, z+1/2'
'-x, z+1/2, -y+1/2'
'z, -y+1/2, -x+1/2'
'-z, -x+1/2, y+1/2'
'-y, -z+1/2, x+1/2'
'-z, -y+1/2, x+1/2'
'z, -x+1/2, y+1/2'
'-x, -z+1/2, y+1/2'
'-y, z+1/2, x+1/2'
'-x, z+1/2, y+1/2'
'z, -y+1/2, x+1/2'
'-x, y+1/2, -z+1/2'
'-y, x+1/2, -z+1/2'
'-x, y+1/2, z+1/2'
'-y, x+1/2, z+1/2'
'y, z+1/2, x+1/2'
'x, y+1/2, -z+1/2'
'y, x+1/2, z+1/2'
'z, x+1/2, y+1/2'
'z, y+1/2, x+1/2'
'-z, x+1/2, y+1/2'
'-x+1/2, -y, -z+1/2'
'-x+1/2, -z, -y+1/2'
'-y+1/2, z, -x+1/2'
'-y+1/2, -x, z+1/2'
'-x+1/2, z, -y+1/2'
'z+1/2, -y, -x+1/2'
'-z+1/2, -x, y+1/2'
'-y+1/2, -z, x+1/2'
'-z+1/2, -y, x+1/2'
'z+1/2, -x, y+1/2'
'-x+1/2, -z, y+1/2'
'-y+1/2, z, x+1/2'
'-x+1/2, z, y+1/2'
'z+1/2, -y, x+1/2'
'-x+1/2, y, -z+1/2'
'-y+1/2, x, -z+1/2'
'-x+1/2, y, z+1/2'
'-y+1/2, x, z+1/2'
'y+1/2, z, x+1/2'
'x+1/2, y, -z+1/2'
'y+1/2, x, z+1/2'
'z+1/2, x, y+1/2'
'z+1/2, y, x+1/2'
'-z+1/2, x, y+1/2'
'-x+1/2, -y+1/2, -z'
'-x+1/2, -z+1/2, -y'
'-y+1/2, z+1/2, -x'
'-y+1/2, -x+1/2, z'
'-x+1/2, z+1/2, -y'
'z+1/2, -y+1/2, -x'
'-z+1/2, -x+1/2, y'
'-y+1/2, -z+1/2, x'
'-z+1/2, -y+1/2, x'
'z+1/2, -x+1/2, y'
'-x+1/2, -z+1/2, y'
'-y+1/2, z+1/2, x'
'-x+1/2, z+1/2, y'
'z+1/2, -y+1/2, x'
'-x+1/2, y+1/2, -z'
'-y+1/2, x+1/2, -z'
'-x+1/2, y+1/2, z'
'-y+1/2, x+1/2, z'
'y+1/2, z+1/2, x'
'x+1/2, y+1/2, -z'
'y+1/2, x+1/2, z'
'z+1/2, x+1/2, y'
'z+1/2, y+1/2, x'
'-z+1/2, x+1/2, y'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
C2 C 0.05392(17) 0.26713(19) 0.19175(16) 0.154(3) Uani 1 1 d U
C1 C 0.0000 0.3120(2) 0.3120(2) 0.122(4) Uani 1 4 d S
S1 S 0.0000 0.34060(7) 0.34060(7) 0.365(5) Uani 1 4 d S
N1 N 0.0000 0.28942(12) 0.28942(12) 0.086(2) Uani 1 4 d S
Co1 Co 0.0000 0.2500 0.2500 0.0735(7) Uani 1 8 d S
N2 N 0.04097(12) 0.27817(11) 0.22183(11) 0.0948(17) Uani 1 2 d S
H2 H 0.0435 0.2468 0.1808 0.185 Uiso 1 1 calc R
C3 C 0.08263(17) 0.28377(18) 0.17459(16) 0.159(3) Uani 1 1 d U
H3 H 0.0919 0.2734 0.1534 0.191 Uiso 1 1 calc R
C4 C 0.09727(15) 0.31326(12) 0.18674(12) 0.0853(19) Uani 1 2 d S
C5 C 0.12608(15) 0.33078(13) 0.16922(13) 0.0930(19) Uani 1 2 d S
N3 N 0.14012(10) 0.35988(10) 0.18431(13) 0.0946(16) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
N1 C1 S1 180.0(9) . .
C1 N1 Co1 180.0(6) . .
N1 Co1 N1 180.00(18) 121 .
N1 Co1 N2 90.0 121 2
N1 Co1 N2 90.0 . 2
N1 Co1 N2 90.000(1) 121 121
N1 Co1 N2 90.0 . 121
N2 Co1 N2 91.6(3) 2 121
N1 Co1 N2 90.0 121 122
N1 Co1 N2 90.0 . 122
N2 Co1 N2 179.995(1) 2 122
N2 Co1 N2 88.4(3) 121 122
N1 Co1 N2 90.0 121 .
N1 Co1 N2 90.000(1) . .
N2 Co1 N2 88.4(3) 2 .
N2 Co1 N2 180.00(18) 121 .
N2 Co1 N2 91.6(3) 122 .
C2 N2 C2 114.6(7) 37 .
C2 N2 Co1 122.7(3) 37 .
C2 N2 Co1 122.7(3) . .
N2 C2 C3 123.1(5) . .
N2 C2 H2 118.5 . .
C3 C2 H2 118.5 . .
C4 C3 C2 122.4(5) . .
C4 C3 H3 118.8 . .
C2 C3 H3 118.8 . .
C3 C4 C3 114.1(6) . 37
C3 C4 C5 123.0(3) . .
C3 C4 C5 123.0(3) 37 .
N3 C5 N3 122.4(6) 176 .
N3 C5 C4 118.7(3) 176 .
N3 C5 C4 118.7(3) . .
C5 N3 C5 117.6(6) 172 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
S1 C1 1.517(12) .
C1 N1 1.194(10) .
N1 Co1 2.089(7) .
Co1 N1 2.088(7) 121
Co1 N2 2.141(5) 2
Co1 N2 2.141(5) 121
Co1 N2 2.141(5) 122
Co1 N2 2.141(5) .
N2 C2 1.294(6) 37
N2 C2 1.294(6) .
C2 C3 1.400(8) .
C2 H2 0.9500 .
C3 C4 1.315(6) .
C3 H3 0.9500 .
C4 C3 1.315(6) 37
C4 C5 1.424(7) .
C5 N3 1.336(3) 176
C5 N3 1.336(3) .
N3 C5 1.336(3) 172
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
S1 C1 N1 Co1 0.0 . .
C1 N1 Co1 N1 0.0 . 121
C1 N1 Co1 N2 0(47) . 2
C1 N1 Co1 N2 0(47) . 121
C1 N1 Co1 N2 0(100) . 122
C1 N1 Co1 N2 0(100) . .
N1 Co1 N2 C2 178.8(6) 121 37
N1 Co1 N2 C2 -1.2(6) . 37
N2 Co1 N2 C2 -91.2(6) 2 37
N2 Co1 N2 C2 61(13) 121 37
N2 Co1 N2 C2 88.8(6) 122 37
N1 Co1 N2 C2 1.2(6) 121 .
N1 Co1 N2 C2 -178.8(6) . .
N2 Co1 N2 C2 91.2(6) 2 .
N2 Co1 N2 C2 -117(13) 121 .
N2 Co1 N2 C2 -88.8(6) 122 .
C2 N2 C2 C3 7.5(13) 37 .
Co1 N2 C2 C3 -174.7(6) . .
N2 C2 C3 C4 -4.2(13) . .
C2 C3 C4 C3 0.2(14) . 37
C2 C3 C4 C5 -178.9(7) . .
C3 C4 C5 N3 -3.5(11) . 176
C3 C4 C5 N3 177.5(7) 37 176
C3 C4 C5 N3 -177.5(7) . .
C3 C4 C5 N3 3.5(11) 37 .
N3 C5 N3 C5 0.1(13) 176 172
C4 C5 N3 C5 173.8(4) . 172
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 -0.003 -0.008 -0.004 40513 13728 ' '
